3) Argillaceous Rocks (CaCO 3 < 40%) Clays Clays Shales Shales Slates Slates Portland cement is made by mixing substances containing CaCO 3 with substances containing SiO 2, Al 2 O 3, Fe 2 O 3 and heating them to a clinker which is subsequently ground to powder and mixed with 2-6 % gypsum.
PRODUCTION STEPS 1) Raw materials are crushed, screemed & stockpiled. 2) Raw materials are mixed with definite proportions to obtain “raw mix”. They are mixed either dry (dry mixing) or by water (wet mixing). 3) Prepared raw mix is fed into the rotary kiln. 4) As the materials pass through the kiln their temperature is rised upto °C. The process of heating is named as “burning”. The output is known as “clinker” which is cm in diameter.
5) Clinker is cooled & stored. 6) Clinker is ground with gypsum (3-6%) to adjust setting time. 7) Packing & marketting.
REACTIONS IN THE KILN ~100°C → free water evaporates. ~100°C → free water evaporates. ~ C°→ loosely bound water is lost from clay. ~ C°→ loosely bound water is lost from clay. ~ °C→decomposition of clay→SiO 2 &Al 2 O 3 ~ °C→decomposition of clay→SiO 2 &Al 2 O 3 ~600°C→decomposition of MgCO 3 →MgO&CO 2 (evaporates) ~600°C→decomposition of MgCO 3 →MgO&CO 2 (evaporates) ~900°C→decomposition of CaCO 3 →CaO&CO 2 (evaporates) ~900°C→decomposition of CaCO 3 →CaO&CO 2 (evaporates)
~ °C →liquid formation & start of compound formation. ~ °C →liquid formation & start of compound formation. ~1280°C→clinkering begins. ~1280°C→clinkering begins. ~ °C→clinkering ~ °C→clinkering ~100°C→clinker leaves the kiln & falls into a cooler. ~100°C→clinker leaves the kiln & falls into a cooler. Sometimes the burning process of raw materials is performed in two stages: preheating upto 900°C & rotary kiln
CHEMICAL COMPOSITION OF P.C. Portland cement is composed of four major oxides (CaO, SiO 2, Al 2 O 3, Fe 2 O 3 ≥90%) & some minor oxides. Minor refers to the quantity not importance.
OxideCommon NameAbbreviationApprox. Amount (%) CaOLimeC60-67 SiO 2 SilicaS17-25 Al 2 O 3 AluminaA3-8 Fe 2 O 3 Iron-oxideF0.5-6 MgOMagnesiaM0.1-4 Na 2 OSodaN K2OK2OPotassaK SO 3 Sulfuric Anhydride Ś 1-3 CaO →limestone CaO →limestone SiO 2 -Al 2 O 3 →Clay SiO 2 -Al 2 O 3 →Clay Fe 2 O 3 →Impurity in Clays Fe 2 O 3 →Impurity in Clays SO 3 →from gypsum→not from the clinker SO 3 →from gypsum→not from the clinker
The amount of oxides in a P.C. Depend on the proportioning of the raw materials and how well the burning is done in the kiln. The chemical composition is found by chemical analysis. A typical analysis of O.P.C. Insoluble residue=0.2 Insoluble residue=0.2 Loss on ignition=1.4 Loss on ignition=1.4 C63.6 S20.7 A6 F2.4 Ś 2.1 M2.6 N0.1 K0.9 Free C1.4 Total99.8
CaO (C), SiO 2 (S), Al 2 O 3 (A) & Fe 2 O 3 are the major oxides that interact in the kiln & form the major compounds. The proportions of these oxides determine the proportions of the compounds which affect the performance of the cement. SO 3 →comes largely from gypsum P.C. alone sets quickly so some gypsum is ground with clinker to retard the setting time.
If too much gypsum is included it leads to distruptive expansions of the hardened paste or concrete. ASTM C 150 → SO 3 ≤ 3% in O.P.C. MgO+HO→MH MgO+H 2 O→MH C+H→CH volume expansion & cause cracking. ASTM C 150 → M<6% free C < 3% free C < 3%
Alkalies (Na 2 O & K 2 O) may cause some dificulties if the cement is used with certain types of reactive aggregates in making concrete. The alkalies in the form of alkaline hydroxides can react with the reactive silica of the aggregate & resulting in volume expansion after hardening. This process may take years. Na 2 O & K 2 O ≤ 0.6%
Insoluble Residue: is that fraction of cement which is insoluble in HCl. It comes mainly from the silica which has not reacted to form compounds during the burning process in the kiln. All compounds of P.C. is soluble in HCl except the silica. The amount of I.R., determined by chemical analysis, serves to indicate the completeness of the reactions in the kiln. ASTM C 150 → I.R. ≤ 0.75%
Loss on Ignition (L.O.I.): is the loss in weight of cement after being heated to 1000°C. It indicates the prehydration or carbonation due to prolonged or improper storage of cement & clinker. If cement is exposed to air, water & CO 2 are absorbed & by heating the cement upto 1000°C loose these two substances. ASTM C 150 → L.O.I. ≤ 3% for O.P.C.
COMPOUND COMPOSITION OF P.C. (OR CLINKER) Oxides interact with eachother in the kiln to form more complex products (compounds). Basically, the major compounds of P.C. can be listed as: NameChemical FormulaAbbreviations Tri Calcium Silicate3CaO.SiO 2 C3SC3S Di Calcium Silicate2CaO.SiO 2 C2SC2S Tri Calcium Aluminate3CaO.Al 2 O 3 C3AC3A Tetra Calcium Alumino Ferrite 4CaO.Al 2 O 3.Fe 2 O 3 C 4 AF
The degree to which the potential reactions can proceed to “equilibrium” depends on: 1) Fineness of raw materials & their intermixing. 2) The temperature & time that mix is held in the critical zone of the kiln. 3) The grade of cooling of clinker may also be effective on the internal structure of major compounds.
There are also some minor compounds which constitute few %, so they are usually negligible. Moreover, portland cement compounds are rarely pure. For example in C 3 S, MgO & Al 2 O 3 replaces CaO randomly. C 3 S →ALITE & C 2 S→BELITE Ferrite Phase: C 4 AF is not a true compound. The ferrite phase ranges from C 2 AF to C 6 AF. *C 4 AF represents an average.
Methods of Determining Compound Composition Each grain of cement consists of an intimate mixture of these compounds. They can be determined by: 1) Microscopy 2) X-Ray Diffraction But due to the variabilities involved the compound composition is usually calculated using the oxide proportions. 3) Calculations (Bouge’s Equations)
Assumptions 1) The chemical reactions in the kiln proceeded to equilibrium. 2) Compounds are in pure form such as C 3 S & C 2 S 3) Presence of minor compounds are ignored. 4) Ferrite phase can be calculated as C 4 AF 5) All oxides in the kiln have taken part in forming the compounds.
Ex:Given the following oxide composition of a portland cement clinker. CaO=64.9% SiO 2 =22.2% Al 2 O 3 =5.8% Fe 2 O 3 =3.1% MgO=4% Using Bogue’s eqn’s calculate the compound composition of the P.C. clinker? Using Bogue’s eqn’s calculate the compound composition of the P.C. clinker? C 3 S=4.071* * * *3.1=52.1% C 2 S=2.876* *52.1=24.5% C 3 A=2.65* *3.1=10.1%
C 4 AF=3.043*3.1=9.4% To see the effect of change in oxide composition on the change in compound composition, assume that CaO is 63.9% & SiO 2 is 23.2% and others are the same. C 3 S=40.4%, C 2 S=36.2%, C 3 A=10%, C 4 AF=9.4% C 3 S changed from 52.1% →40.4% C 2 S changed from 24.5%→36.2% 1% change in CaO & SiO 2 resulted in more than 10% change in C 3 S & C 2 S content.
Influence of Compound Composition on Characteristics of P.C. P.C.+water →the compounds in the cement undergo chemical reactions with the water independently, and different products result from these reactions. C3SC3SC2SC2SC3AC3AC 4 AF Rate of ReactionModerateSlowFastModerate Heat LiberationHighLowVery HighModerate Early Cementitious ValueGoodPoorGoodPoor Ultimate Cementitious ValueGood Poor
ASTM Type & Name of P.C. Average Compound Composition C3SC3SC2SC2SC3AC3AC 4 AF Type I - O.P.C General Purpose Type II - Modified For Moderate Heat of Hydration Type III - High Early Strength C 3 S&C 3 A increased, C 2 S decreased Type IV - Low Heat P.C C 2 S increased Type V - Sulfate Resistant P.C Limit on C 3 A≤5%, 2C 3 A+C 4 AF≤25%
Hydration of P.C. Hydration: Chemical reactions with water. As water comes into contact with cement particles, hydration reactions immediately starts at the surface of the particles. Although simple hydrates such as C-H are formed, process of hydration is a complex one and results in reorganization of the constituents of original compounds to form new hydrated compounds.
At any stage of hydration the hardened cement paste (hcp) consists of: Hydrates of various compounds referred to collectively as GEL. Hydrates of various compounds referred to collectively as GEL. Crystals of calcium hydroxide (CH). Crystals of calcium hydroxide (CH). Some minor compound hydrates. Some minor compound hydrates. Unhydrated cement Unhydrated cement The residual of water filled spaces – pores. The residual of water filled spaces – pores.
As the hydration proceeds the deposits of hydrated products on the original cement grains makes the diffusion of water to unhydrated nucleus more & more difficult. Thus, the rate of hydration decreases with time & as a result hydration may take several years. Major compounds start to produce: Calcium-silicate-hydrate gels Calcium-silicate-hydrate gels Calcium hydroxide cement Calcium hydroxide cement Calcium-alumino-sulfohydrates gel Calcium-alumino-sulfohydrates gel
At the beginning of mixing, the paste has a structure which consists of cement particles with water-filled space between them. As hydration proceeds, the gels are formed & they occupy some of this space. 1cc of cement → 2.1cc of gel Gel Pores: 28% of the total gel volume have diameter of μm. (very small-loss or gain of water is difficult)
Capillary Pores: 12.5 μm diameter, with varying sizes, shapes & randomly distributed in the paste. Volume of capillary pores decreases as hydration takes place. Water in capillary pores is mobile, can not be lost by evaporation or water can get into the pores. They are mainly responsible for permeability. - w/c ratio capillary porosity capillary porosity - degree of hydration - degree of hydration
C 2 S & C 3 S: 70-80% of cement is composed of these two compounds & most of the strength giving properties of cement is controlled by these compounds. Upon hydration both calcium-silicates result in the same products. 2C 3 S+6H → C 3 S 2 H 3 + 3CH 2C 2 S+4H → C 3 S 2 H 3 + CH Calcium-Silicate-Hydrate (C-S-H gel) is similar to a mineral called “TOBERMORITE”. As a result it is named as “TOBERMORITE GEL”
Upon hydration C 3 S & C 2 S, CH also forms which becomes an integral part of hydration products. CH does not contribute very much to the strength of portland cement. C 3 S having a faster rate of reaction accompanied by greater heat generation developes early strength of the paste. On the other hand, C 2 S hydrates & hardens slowly so results in less heat generation & developes most of the ultimate strength.
Higher C 3 S →higher early strength-higher heat generation (roads, cold environments) Higher C 2 S→lower early strength-lower heat generation (dams) C 3 A: is characteristically fast reacting with water & may lead to a rapid stiffening of the paste with a large amount of the heat generation (Flash-Set)-(Quick-Set). In order to prevent this rapid reaction gypsum is added to the clinker. Gypsum, C 3 A&water react to form relatively insoluble Calcium- Sulfo-Aluminates.
C 3 A+CŚH 2 +10H →C 4 A ŚH 12 (calcium- alumino- monosulfohydrate) C 3 A+3CŚH 2 +26H →C 6 A Ś 3 H 32 (calcium-alumino- trisulfohydrate “ettringite”) When there is enough gypsum “ettringite” forms with great expansion If there is no gypsum →flash-set more gypsum→ettringite more gypsum→ettringite formation increases formation increases which will cause cracking which will cause cracking
Also Calcium-Sulfo Aluminates are prone (less resistant) to sulfate attack & does not contribute much for strength. The cement to be used in making concretes that are going to be exposed to soils or waters that contain sulfates should not contain more than 5% C 3 A. C 4 AF: The hydration of ferrite phase is not well understand. Ferrite phase has lesser role in development of strength. The hydration products are similar to C 3 A. Alumina & iron oxide occur interchangebly in the hydration products. C 4 AŚH 12 or C 4 FŚH 12 C 6 AŚ 3 H 32 or C 6 FŚ 3 H 32
HEAT OF HYDRATION Hydration process of cement is accompanied by heat generation (exothermic). As concrete is a fair insulator, the generated heat in mass concrete may result in expansion & cracking. This could be overcome by using suitable cement type. It could also be advantages for cold wheather concreting. The heat of hydration of OPC is on the order of cal/gr. About 50% of this heat is liberatedwithin 1-3 days & 75% within 7 days. By limiting C 3 S&C 3 A content heat of hydration can be reduced.
Heat of Hydration of Pure Compounds Heat of Hydration (cal/gr) C3SC3S120 C2SC2S62 C3AC3A207 C 4 AF100 The amount of heat liberated is affected by the fractions of the compounds of the cement. Heat of Hydration(cal/gr)=120 *(%C 3 S)+62*(%C 2 S)+ 207*(%C 3 A)+100*(C 4 A F)
FINENESS OF CEMENT As hydration takes place at the surface of the cement particles, it is the surface area of cement particles which provide the material available for hydration. The rate of hydration is controlled by fineness of cement. For a rapid rate of hydration a higher fineness is necessary.
However, Higher fineness requires higher grinding (cost ) Higher fineness requires higher grinding (cost ) Finer cements deteriorate faster upon exposure to atmosphere. Finer cements deteriorate faster upon exposure to atmosphere. Finer cements are very sensitive to alkali- aggregate reaction. Finer cements are very sensitive to alkali- aggregate reaction. Finer cements require more gypsum for proper hydration. Finer cements require more gypsum for proper hydration. Finer cements require more water. Finer cements require more water.
Fineness of cement is determined by air permeability methods. For example, in the Blaine air permeability method a known volume of air is passed through cement. The time is recorded and the specific surface is calculated by a formula. Fineness is expressed in terms of specific surface of the cement (cm 2 /gr). For OPC specific surface is cm 2 /gr.
Blaine Apparatus Sieving
SETTING Setting refers to a change from liquid state to solid state. Although, during setting cement paste acquires some strength, setting is different from hardening. The water content has a marked effect on the time of setting. In acceptance tests for cement, the water content is regulated by bringing the paste to a standard condition of wetness. This is called “normal consistency”.
Normal consistency of O.P.C. Ranges from % by weight of cement. Vicat apparatus is used to determine normal consistency. Normal consistency is that condition for which the penetration of a standard weighed plunger into the paste is 10mm in 30sec. By trial & error determine the w/c ratio. In practice, the terms initial set&final set are used to describe arbitrary chosen time of setting. Initial set indicates the beginning of a noticeable stiffening & final set may be regarded as the start of hardening (or complete loss of plasticity).
Vicat Needle Gillmore Needle
Setting can be obtained by using the vicat apparatus. Initial setting time>45min Initial setting time>45min ASTM C150 Final setting time<375min Final setting time<375min Initial > 1hr (60min) Initial > 1hr (60min) TS 19 Final < 8hr (480min) Final < 8hr (480min)
Factors Affecting Setting Time Temperature & Humidity Temperature & Humidity Amount of Water Amount of Water Chemical Composition of Cement Chemical Composition of Cement Fineness of Cement (finer cement, faster setting) Fineness of Cement (finer cement, faster setting) Flash-set Flash-set Abnormal Settings False-set False-set
Flash-Set: is the immediate stiffening of cement paste in a few minutes after mixing with water. It is accompanied by large amount of heat generation upon reaction of C3A with water. Gypsum is placed in cement to prevent flash- set. The rigidity can not be overcome & plasticity may not be regained without addition of water. Amount of gypsum must be such that it will be used upto almost hardening. Because expansion caused by ettringite can be distributed to the paste before hardening. More gypsum will cause undesirable expansion after hardening.
False-Set: is a rapid development of rigidity of cement paste without generation of much heat. This rigidity can be overcome & plasticity can be regained by further mixing without addition of water. In this way cement paste restores its plasticity & sets in a normal manner without any loss of strength. Probable Causes of False-Set: 1) When gypsum is ground by too hot of a clinker, gypsum may be dehydrated into hemihydrate (CaSO 4.1/2H 2 O) or anhydrate (CaSO 4 ). These materials when react with water gypsum is formed, which results in stiffening of the paste.
2) Alkali oxides in cement may carbonate during storage. Upon mixing such a cement with water, these alkali carbonates will react with Ca(OH 2 ) (CH-Calcium Hydroxide) liberated by hydrolysis of C 3 S resulting in CaCO 3. CaCO 3 precipates in the mix & results in false-set.
SOUNDNESS OF CEMENT Soundness is defined as the volume stability of cement paste. The cement paste should not undergo large changes in volume after it has set. Free CaO&MgO may result in unsound cement. Upon hydration C&M will form CH&MH with volume increase thus cracking. Since unsoundness is not apparent until several months or years, it is necessary to provide an accelerated method for its determination. 1) Lechatelier Method: Only free CaO can be determined. 2) Autoclave Method: Both free CaO&MgO can be determined.
STRENGTH OF CEMENT Strength tests are not carried out on neat cement pastes, because it is very difficult to form these pastes due to cohesive property of cement. Strength tests are carried out on cement mortar prepared by standard gradation (1 part cement+3 parts sand+1/2 part water)
1) Direct Tension (Tensile Strength): σ t =P/1in 2 σ t =P/1in 2 Difficult test procedure Difficult test procedure P P 1”
2) Flexural Strength (tensile strength in bending): σf=(M*C)/I σf=(M*C)/I M:maximum moment M:maximum moment I:moment of inertia I:moment of inertia C:distance to bottom fiber from C.G. C:distance to bottom fiber from C.G. P L 4 cm C
3) Compression Test: i) Cubic Sample ii)Flexural Sample after it is broken P P σ c =P/A 4 cm σ c =P/A A=4x4
TYPES OF PORTLAND CEMENT Cements of different chemical composition & physical characteristics may exhibit different properties when hydrated. It should thus be possible to select mixtures of raw materials for the production of cements with various properties. In fact several cement types are available and most of them have been developed to ensure durability and strength properties to concrete.
It should also be mentioned that obtaining some special properties of cement may lead to undesirable properties in another respect. For this reason a balance of requirements may be necessary and economic aspects should be considered. 1) Standard Types: these cements comply with the definition of P.C., and are produced by adjusting the proportions of four major compounds. 2) Special Types: these do not necessarily couply with the definiton of P.C. & are produced by using additional raw materials.
Standard Cements (ASTM) Type I: Ordinary Portland Cement Suitable to be used in general concrete construction when special properties are not required. Type II: Modified Portland Cement Suitable to be used in general concrete construction. Main difference between Type I&II is the moderate sulfate resistance of Type II cement due to relatively low C3A content (≤%8). Since C 3 A is limited rate of reactions is slower and as a result heat of hydration at early ages is less. *It is suitable to be used in small scale mass concrete like retaining walls.
Type III: High Early Strength P.C. Strength development is rapid. 3 days f’ c =7 days f’ c of Type I It is useful for repair works, cold weather & for early demolding. Its early strength is due to higher C 3 S & C 3 A content. Type IV: Low Heat P.C. Generates less heat during hydration & therefore gain of strengthis slower. In standards a maximum value of C 3 S&C 3 A& a minimum value for C 2 S are placed. It is used in mass-concrete and hot-weather concreting.
Type V: Sulfate Resistant P.C. Used in construction where concrete will be subjected to external sulfate attack – chemical plants, marine & harbor structures. i) During hydration C 3 A reacts with gypsum & water to form ettringite. In hardened cement paste calcium-alumino-hydrate can react with calcium&alumino sulfates, from external sources, to form ettringite which causes expansion & cracking. ii) C-H and sulfates can react & form gypsum which again causes expansion & cracking. * In Type V C 3 A is limited to 5%.
Type IA, IIA, IIIA: Air Entrained Portland Cement Only difference is adding an air-entraining agent to the cement during manufacturing to increase freeze-thaw resistance by providing small sized air bubbles in concrete.
SPECIAL CEMENTS Portland Pozzolan Cement (P.P.C.) By grinding & blending P.C. Clinker+Pozzolan+Gypsum By grinding & blending P.C. Clinker+Pozzolan+Gypsum P.P.C. Produces less heat of hydration & offers higher sulfate resistance so it can be used in marine structures & mass concrete. P.P.C. Produces less heat of hydration & offers higher sulfate resistance so it can be used in marine structures & mass concrete. However, most pozzolans do not contribute to strength at early ages. However, most pozzolans do not contribute to strength at early ages. The early strength of PPC is less. The early strength of PPC is less.
Portland Blast Furnace Slag Cement (P.B.F.S.C.) By intergrinding B.F.S.+P.C. Clinker+Gypsum By intergrinding B.F.S.+P.C. Clinker+Gypsum This cement is less reactive (rate of gain of strength & early strength is less but ultimate strength is same) This cement is less reactive (rate of gain of strength & early strength is less but ultimate strength is same) High sulfate resistance High sulfate resistance Suitable to use in mass concrete construction Suitable to use in mass concrete construction Unsuitable for cold weather concreting Unsuitable for cold weather concreting Both P.P.C.&P.B.F.S.C. Are called blended cements. Their heat of hydration & strength development are low in early days. Because upon adding water C 3 S compounds start to produce C-S-Hgels & CH. The Ch & the pozzolanic material react together to produce new C-S-H gels. That’s why the early strength is low but the ultimate strength is the same when compared to O.P.C.
White Portland Cement W.P.C. İs made from materials containing a little iron oxide & manganese oxide. W.P.C. İs made from materials containing a little iron oxide & manganese oxide. Fe 2 O 3 + MnO ≤ 0.8% Fe 2 O 3 + MnO ≤ 0.8% To avoid contamination by coal ash, oil is used as fuel. To avoid contamination by coal ash, oil is used as fuel. To avoid contamination by iron during grinding, instead of steel balls nickel- molybdenum alloys are used. To avoid contamination by iron during grinding, instead of steel balls nickel- molybdenum alloys are used.
High Alumina Cement The raw materials for H.A.C. İs limestone and Bauxite (Al 2 O 3 & Fe 2 O 3 ) The raw materials for H.A.C. İs limestone and Bauxite (Al 2 O 3 & Fe 2 O 3 ) These raw materials are interground & introduced in the kiln clinkered at 1600°C. Then the obtained material is ground to a fineness of cm2/gr. These raw materials are interground & introduced in the kiln clinkered at 1600°C. Then the obtained material is ground to a fineness of cm2/gr. The oxide composition is quite different The oxide composition is quite different Al 2 O 3 → 40-45% CaO → 35-42% Fe 2 O 3 → 5-15% SiO 2 → 4-10%
Major compounds are CA & C2S Major compounds are CA & C2S It is basically different from O.P.C. & the concrete made from this cement has very different properties. It is basically different from O.P.C. & the concrete made from this cement has very different properties. It has high sulfate resistance. It has high sulfate resistance. Very high early strength (emergency repairs) Very high early strength (emergency repairs) About 80% of ultimate strength is obtained within 24 hours. But the strength is adversely affected by temperature. The setting time is not as rapid as gain of strength. About 80% of ultimate strength is obtained within 24 hours. But the strength is adversely affected by temperature. The setting time is not as rapid as gain of strength. Initial setting time is 4 hrs & final setting time is 5 hrs. Initial setting time is 4 hrs & final setting time is 5 hrs.
STANDARD TURKISH CEMENTS (TS 19) – Cancelled TS 19 groups them into 3 P.Ç → min. Compressive strength is 32.5 MPa in 28 days. P.Ç P.Ç Special Cements are: TS 20 –Blast Furnace Slag Cement CÇ 32.5 – Cüruflu Çimento CÇ 42.5 TS 21 – White Portland Cement BPÇ TS22 – Masonry Cement, HÇ 16 (Harç Çimentosu) TS 26 – Trass Cement, TÇ 32.5 (Traslı Çimento) TS 640 – Fly Ash Cement, UKÇ 32.5 (Uçucu Küllü Çimento)
TS EN NEW CEM cements CEM I – Portland Cement CEM II – Portland Composite Cement CEM III – Portland Blast Furnace Slag Cement CEM IV – Pozzolanic Cement CEM V – Composite Cement 27 different cements
TS EN CEM cements : CEM cements : –Binding property is mainly due to hydration of calcium-silicates –Reactive C + Reactive S > 50% Clinker, major and minor mineral admixtures Clinker, major and minor mineral admixtures –Clinker + Major + Minor = 100% (mass) + Gypsum –Major > 5% by mass –Minor 5% by mass
TS EN Mineral Admixtures K : Clinker K : Clinker D : Silica Fume D : Silica Fume P : Natural Pozzolan P : Natural Pozzolan Q : Calcined Natural Pozzolan Q : Calcined Natural Pozzolan T : Calcined Shale T : Calcined Shale W : Class – C Fly Ash W : Class – C Fly Ash V : Class – F Fly Ash V : Class – F Fly Ash L : Limestone (Organic compound < 0.5%) L : Limestone (Organic compound < 0.5%) LL : Limestone (Organic compound < 0.2%) LL : Limestone (Organic compound < 0.2%) S : Granulated Blast Furnace Slag S : Granulated Blast Furnace Slag
TS EN Composition A : Lowest amount of mineral admixture A : Lowest amount of mineral admixture B : Mineral admixture amount is > A B : Mineral admixture amount is > A C : Mineral admixture amount is > B C : Mineral admixture amount is > B
TS EN Composition CEM I : Portland Cement CEM I : Portland Cement % K + 0-5% Minor
TS EN Composition CEM II : Portland Composite Cement CEM II : Portland Composite Cement CEM II/A-S : Portland Slag Cement 80-94% K % S + 0-5% Minor CEM II/B-S : Portland Slag Cement 65-79% K % S + 0-5% Minor CEM II/B-P : Portland Pozzolanic Cement 65-79% K % P + 0-5% Minor CEM II/A-V : Portland Fly Ash Cement 80-94% K % V + 0-5% Minor
TS EN Composition CEM III : CEM III : Portland Blast Furnace Slag Cement CEM III/A : Portland Blast Furnace Slag Cement 35-64% K % S + 0-5% Minor CEM III/B : Portland Blast Furnace Slag Cement 20-34% K % S + 0-5% Minor CEM III/C : Portland Blast Furnace Slag Cement 5-19% K % S + 0-5% Minor
TS EN Composition CEM IV : CEM IV : Pozzolanic Cement CEM IV/A : Pozzolanic Cement 65-89% K % (D,P,Q,V,W) + 0-5% Minor CEM IV/B : Pozzolanic Cement 45-64% K % (D,P,Q,V,W) + 0-5% Minor
TS EN Composition CEM V : Composite CEM V : Composite Cement CEM V/A : Composite Cement 40-64% K % S % (P,Q,V) + 0-5% Minor CEM V/B : Composite Cement 20-38% K % S % (P,Q,V) + 0-5% Minor
Name - Example CEM II / A – P 42.5 N CEM II / A – P 42.5 N CEM II / A – P 42.5 R CEM II / A – P 42.5 R